Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Electrical resistivity and conductivity wikipedia, lookup

Transcript
```Chapter
3
SEMICONDUCTOR
BANDSTRUCTURE
In this chapter we present gures discussing bandstructures of important semiconductors and the
concept of doping and mobile carriers.
SEMICONDUCTOR BANDSTRUCTURE
In semiconductors we are pimarily interested in the
valence band and conduction band. Moreover, for
most applications we are interested in what happens
near the top of the valence band and the bottom of
the conduction band. These states originate from the
atomic levels of the valence shell in the elements
making up the semiconductor.
IV Semiconductors
C
1s22s22p2
Si
1s22s22p63s23p2
Ge
1s22s22p63s23p63d104s24p2
III-V Semiconductors
Ga
1s22s22p63s23p63d104s24p1
As
1s22s22p63s23p63d104s24p3
Outermost atomic levels are either s-type or p-type.
www.eecs.umich.edu/~singh
BANDSTRUCTURE OF SEMICONDUCTORS
The k-vector for the electrons in a crystal is limited to a
space called the Brillouin zone. The figure shows the
Brillouin zone for the fcc lattice relevant for most
semiconductors. The values and notations of certain
important k-points are also shown. Most semiconductors
have bandedges of allowed bands at one of these points.
IMPORTANT HIGH SYMMETRY POINTS
Γ point: kx = 0 = ky = kz
L
Γ
X point: kx = 2π ; ky = kz = 0
a
L point: kx = ky = kz = π
a
a = lattice constant (cube edge)
X
A TYPICAL BANDSTRUCTURE: Si
6
4
ENERGY (eV)
2
Γ2
L3
L1
Γ2
Γ15
Γ25
Γ15
Γ25
0 L
3
Χ1
Χ4
–2
–4
–6
–8 L1
L
–10 2
Γ1
–12
L
Λ
Γ
Γ1
∆
Χ UK
Σ
Γ
www.eecs.umich.edu/~singh
BANDSTRUCTURE NEAR BANDEDGES
Behavior of electrons near the bandedges determines most device
properties. Near the bandedges the electrons can be described by
simple effective mass pictures, i.e., the electrons behave as if they
are in free space except their masses are m*.
DIRECT
CONDUCTION
BAND
AAA
AAA
AAA
AAA
AAA
AA
A
AA
AA
AAA
AA
AAA
AAA
A
A
AA
AAA
AAA
INDIRECT
CONDUCTION
BAND
Direct
bandgap
Indirect
bandgap
∆
I
II
VALENCE
BAND
III
I
Heavy Hole Band
II Light Hole Band
III Split-Off Band
∆ = Split-Off Energy
k=0
k
Schematic of the valence band, direct bandgap, and indirect bandgap
conduction bands. The conduction band of the direct gap
semiconductor is shown in the solid line, while the conduction band
of the indirect semiconductor is shown in the dashed line. The
curves I, II, and III in the valence band are called heavy hole, light
hole, and split-off hole states, respectively.
www.eecs.umich.edu/~singh
EFFECTIVE MASS DESCRIPTION
CONDUCTION BAND: Direct bandgap material
h2k2
Ec(k) = Ec(0) + 2m*c
with
2 1
2pcv
1
2 +
1
= 1 +
2
m*
m
3
E
m
E
c
gΓ + ∆
gΓ
(
)
The smaller the bandgap, the smaller the effective mass.
h2k2
Eso = –∆ – 2m*so
SPLIT-OFF BAND:
2
2pcv
1
= –1 +
m*so
m
(3m2EgΓ + ∆)
HEAVY HOLE; LIGHT HOLE:
In a simple approximation the heavy hole and light hole bands can
also be represented by masses m*hh and m* h. However, the real
picture is more complex.
CdS
AlAs
AlSb
ZnTe
GaP
ZnSe
EFFECTIVE MASS
*
( mmoc )
0.2
CdSe
CdTe
InP
GaAs
0.1
GaSb
0
InAs
InSb
1.0
0
BANDGAP
2.0
Eg (eV)
www.eecs.umich.edu/~singh
3.0
BANDSTRUCTURE: SILICON
Although the bandstructure of Si is far from ideal, having an indicrect bandgap, hig hhole masses,
and small spin-orbit splitting, processing related advantages make Si the premier semiconductor
for consumer electronics. On the right we show constant energy ellipsoids for Si conduction band.
There are six equivalent valleys in Si at the bandedge.
Silicon
6
Eg = 1.1eV
5
at 300K
kz
ENERGY (eV)
4
(001)
3
2
3.4
Six equivalent
valleys at
(100)
conduction
bandedge
1.1
(010)
1
Eg
0
(100)
kx
–1
(010)
(001)
–2
–3
Eg = 1.17 –
–4
4.37 x 10–4 T2
(eV)
T – 636
ky
T = Temperature in K
k
(b)
(a)
• Indirect gap material
weak optical transitions, cannot be used to produce lasers.
2π
2π
• Valleys along the x-axis and –x-axis: k0x = a (0.85,0,0) and k0x = a (–0.85,0,0):
(kx – k0x)2
kx2 + kz2
; ml = 0.98 m0; mt = 0.19 m0
+
m*l
m*t
similar E-k relations for other 4 valleys.
2
E(k) = Ec + h
2
• Density of states mass = 1.08 m0 (6 valleys included).
• Heavy hole mass: 0.49 m0 ; light hole mass: 0.16 m0.
• Intrinsic carrier concentration at 300 K: 1.5 x 1010 cm–3.
www.eecs.umich.edu/~singh
BANDSTRUCTURE: GaAs
The bandgap at 0 K is 1.51 eV and at 300 K it is 1.43 eV. The bottom of the conductionband
is at k = (0,0,0), i.e., the G-point. The upper conduction band valleys are at the L-point.
Gallium Arsenide
6
Eg = 1.43eV
at 300 K
5
CONDUCTION
BAND
ENERGY (eV)
4
3
2
0.58
0.3
1
Eg
Eg = 1.519 –
0
5.4 x 10–4 T2
(eV)
T + 204
T = Temperature in K
–1
–2
–3
–4
[111]
[100]
k
CONDUCTION BAND:
• Electron mass is light.
m* = 0.067 m0
• Upper valley mass is large. m* = 0.25 m0 results in negative
differential resistance at higher fields.
• Material is direct bandgap and has strong optical transistions
can be used for light emission.
VALENCE BAND:
• Heavy hole mass: 0.45 m0; light hole mass = 0.08 m0.
Intrinsic carrier concentration at 300 = 1.84 x 106 cm–3.
www.eecs.umich.edu/~singh
BANDSTRUCTURE: Ge AlAs, InAs, InP
Germanium
Aluminum Arsenide
6
6
Eg = 0.66eV
at 300K
4
4
3
3
2
0.3
1
0
0.90
2
0
–1
–2
–2
–3
–3
L [111] Γ [100]X
–4
(b)
Indium Arsenide
Indium Phosphide
4
3
3
2
1
0
(c)
E
g
2
1
–1
–2
–2
–3
–3
–4
(d)
0.9
4
0.6
9
Eg
0
–1
L [111] Γ [100]X
k
Eg = 1.34eV
at 300K
5
ENERGY
(eV)
ENERGY
(eV)
Eg = 0.35eV
at 300K
4
–4
L [111] Γ [100]X
6
6
5
Eg
2.75
1
–1
–4
(a)
Eg
Eg = 2.15eV
at 300K
5
ENERGY
(eV)
ENERGY
(eV)
5
L [111] Γ [100]X
k
(a) Bandstructure of Ge. (b) Bandstructure of AlAs. (c) Bandstructure of InAs.
Since no adequate substitute matches InAs directly, it is often used as an alloy
(InGaAs, InAlAs, etc.,) for devices. (d) Bandstructure of InP. InP is a very
important material for high speed devices as well as a substrate and barrier layer
material for semiconductor lasers.
www.eecs.umich.edu/~singh
ELECTRONIC PROPERTIES OF SOME SEMICONDUCTORS
Material
Bandgap
(eV)
Relative
Dielectric
Constant
Material
C
5.5, I
5.57
AlAs
0.1
Si
1.124, I
11.9
AlSb
0.12
* = 0.98
mdos
Ge
0.664, I
16.2
GaN
0.19
* = 0.60
mdos
SiC
2.416, I
9.72
GaP
0.82
* = 0.60
mdos
GaAs
1.424, D
13.18
GaAs
0.067
AlAs
2.153, I
10.06
m*lh = 0.082
m*hh = 0.45
InAs
0.354, D
15.15
GaSb
0.042
* = 0.40
mdos
GaP
2.272, I
11.11
Ge
InP
1.344, D
12.56
InSb
0.230, D
16.8
CdTe
1.475, D
10.2
AlN
6.2, D
9.14
GaN
3.44, D
10.0
ZnSe
2.822, D
9.1
ZnTe
2.394, D
8.7
Electron
Mass
(m0)
ml = 1.64
mt = 0.082
mdos= 0.56
Hole
Mass
(m0)
* = 0.044
mlh
m*hh = 0.28
InP
0.073
* = 0.64
mdos
InAs
0.027
* = 0.4
mdos
InSb
0.13
m*dos = 0.4
Si
ml = 0.98
mt = 0.19
mdos= 1.08
m*lh = 0.16
* = 0.49
mhh
Properties of some semiconductors. D and I stand for direct and indirect gap,
respectively. The data are at 300 K. Note that Si has six conducton band
valleys, while Ge has four.
www.eecs.umich.edu/~singh
SOME IMPORTANT PROPERTIES OF Si AND GaAs
PROPERTY
SI
GAAS
Electron
effective mass
(m0)
m*l = 0.98
m*t = 0.19
m*dos = 1.08
m*σ = 0.26
m* = 0.067
Hole
effective mass
(m0)
m*hh = 0.49
m*lh = 0.16
m*dos = 0.55
m*hh = 0.45
m*lh = 0.08
m*dos = 0.47
Bandgap
(eV)
1.17 – 4.37 x 10–4 T2
T + 636
1.519 – 5.4 x 10–4 T2
T + 204
Electron affinity
(eV)
4.01
4.07
For Si: m*dos: To be used in calculating density of states, position of Fermi level
m*σ: To be used in calculating response to electric field, e.g., in mobility
www.eecs.umich.edu/~singh
HOLES IN SEMICONDUCTORS: WHAT ARE HOLES?
In a filled band (valence band) no current can flow, since electrons are
normally Fermi particles and obey the Pauli exclusion principle. The
electrons can “move” if there is an empty state available. The empty
states in the valence band are called holes.
E
Conduction
band
Wavevector associated
with the missing electron
kh
ke
k
Electron
removed
+
VALENCE
BAND
Missing electron = hole
Diagram illustrating the wavevector of the missing electron ke. The
wavevector of the system with the missing electron is –ke, which is
associated with the hole.
www.eecs.umich.edu/~singh
HOLES IN SEMICONDUCTORS: HOW DO HOLES MOVE?
Holes behave as if they carry a positive charge.
t2 > t1>0
t=0
t = t1
Ε
Ε
Fx
F
E
D
G
C
B
A
t = t2
F
kx
D
H
I
J
K
Ε
Fx
E
G
C
B
A
kx
H
I
J
K
E
D
G
C
B
A
kx
H
I
J
K
(c)
(b)
(a)
Fx
F
F
ve
e
je
vh
h
jh
(d)
The movement of an empty electron state, i,e,. a hole under an electric
field. The electrons move in the direction opposite to the electric field
so that the hole moves in the direction of the electric field thus behaving
as if it were positively charged, as shown in (a), (b), and (c). (d) The
velocities and currents due to electrons and holes. The current flow is in
the same direction, even though the electron and holes have opposite
velocities. The electron effective mass in the valence band is negative,
but the hole behaves as if it has a positive mass.
www.eecs.umich.edu/~singh
FREE CARRIERS IN SEMICONDUCTORS: INTRINSIC CARRIERS
In semiconductors, at finite temperatures, there are electrons in the conduction band
and holes in the valence band.
METALS
Evac
ENERGY
EF
Ec
Electrons in the
conduction band
can carry current
(a)
SEMICONDUCTORS
Evac
ENERGY
–
–
Ec
Electrons in the conduction band
(density, n) carry current
Mobile carrier density = n + p
+ + + EV
Holes in the valence band (density, p)
carry current
Valence band
(b)
(a) A schematic showing allowed energy bands in electrons in a metal. The
electrons occupying the highest partially occupied band are capable of
carrying current. (b) A schematic showing the valence band and conduction
band in a typical semiconductor. In semiconductors only electrons in the
conduction band holes in the valence band can carry current.
For small electron (n), hole (p) densities we can use Boltzmann approximation:
n = Nc exp [(EF– Ec)/kBT]
where
Nc = 2
p=2
m*ekBT 3/2
2πh2
( )
m*hkBT 3/2
exp [(Ev– EF)/kBT]
2πh2
( )
= Nv exp [(Ev– EF)/kBT]
Intrinsic case:
ni = pi = 2
kBT 3/2
(m*em*h)3/4 exp (–Eg/2kBT)
2πh2
( )
www.eecs.umich.edu/~singh
INTRINSIC CARRIER DENSITIES FOR SOME SEMICONDUCTORS
1019
1000 500
T(°C)
200 100
27 0 –20
INTRINSIC CARRIER DENSITY ni (cm–3)
1018
1017
Ge
1016
1015
Temperature dependence of
ni, pi in Si, Ge, GaAs
Si
1014
1013
1012
11
10
10
10
109
GaAs
10 8
10 7
106
0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0
1000/T (K–1)
MATERIAL
CONDUCTION BAND
EFFECTIVE DENSITY (NC )
VALENCE BAND
EFFECTIVE DENSITY (NV )
INTRINSIC CARRIER
CONCENTRATION
Si (300 K)
2.78 x 1019 cm–3
9.84 x 1018 cm–3
1.5 x 1010 cm–3
Ge (300 K)
1.04 x 1019 cm–3
6.0 x 1018 cm–3
2.33 x 1013 cm–3
GaAs (300 K)
4.45 x 1017 cm–3
7.72 x 1018 cm–3
1.84 x 106 cm–3
(ni = pi)
Effective densities and intrinsic carrier concentrations of Si, Ge and GaAs. The numbers for
intrinsic carrier densities are the accepted values even though they are smaller than the values
obtained by using the equations derived in the text.
www.eecs.umich.edu/~singh
DOPING OF SEMICONDUCTORS: DONORS AND ACCEPTORS
If an impurity atom replaces a host semiconductor atom in a crystal it could donate (donor) an
extra electron to the conduction band or it could accept (acceptor) an electron from the valence
band producing a hole.
All 4 outer
electrons go into
the valence band
EC
EV
Silicon
host atom
=
+
+
Electron-ion
Coulombic
Pentavalent
donor impurity = Silicon-like + attraction
A schematic showing the approach one takes to understand donors in semiconductors. The
donor problem is treated as the host atom problem together with a Coulombic interaction term.
The silicon atom has four “free” electrons per atom. All four electrons are contributed to the
valence band at 0 K. The dopant has five electrons out of which four are contribted to the
valence band, while the fifth one can be used for increasing electrons in the conducton band.
E
Si
Si
n-type
silicon
Si
Si
Ec
+
Excess
Donor
As
Si
positive
level
charge
–
Si
Si
Ev
Excess electron
Arsenic (As) atom donates one
electron to the conduction band to
produce an n-type silicon
Conduction
band
Ed
AAAA
AAAA
AAAA
( )( εεso )2 eV
m*
Ed = Ec –13.6 m
o
Valence
band
Charges associated with an arsenic impurity atom in silicon. Arsenic has five valence electrons,
but silicon has only four valence electrons. Thus four electrons on arsenic form tetrahedral
covalent bonds similar to silicon, and the fifth electron is available for conduction. The arsenic
atom is called a donor because when ionized it donates an electron to the conduction band.
www.eecs.umich.edu/~singh
FREE CARRIERS IN DOPED SEMICONDUCTORS
If electron (hole) density is measured as a function of temperature in a doped semiconductor, one
observes three regimes:
Freezeout: Temperature is too small to ionize the donors (acceptors), i.e.,
kBT < EC – ED (kBT< ED – EV).
Saturation: Most of the donors (acceptors) are ionzed.
Intrinsic: Temperature is so high that ni > doping density.
TEMPERATURE (K)
10 17
500
1000 300
200
100
75
50
Si
ELECTRON DENSITY n (cm–3)
Nd = 1015cm–3
Intrinsic range
10 16
Saturation range
10 15
10
Freeze-out
range
14
ni
10 13
0
4
8
12
16
20
1000/T (K–1)
Electron density as a function of temperature for a Si sample with donor impurity
concentration of 1015 cm–3. It is preferable to operate devices in the saturation region
where the free carrier density is approximately equal to the dopant density.
It is not possible to operate devices in the intrinsic regime, since the devices always have a high
carrier density that cannot be controlled by electric fields.
every semiconductor has an upper temperature beyond which it cannot be used in devices.
The larger the bangap, the higher the upper limit.
www.eecs.umich.edu/~singh
Zinc Blende and Wurtzite
CRYSTAL
STATIC
MATERIAL STRUCTURE BANDGAP DIELECTRIC
(EV)
CONSTANT
C
Si
SiC
Ge
BN
DI
DI
ZB
DI
HEX
5.50, I
1.1242, I
2.416, I
0.664, I
5.2, I
BN
BP
BAs
AlN
ZB
ZB
ZB
W
6.4, I
2.4, I
—
6.2,D
AlP
AlAS
AlSb
GaN
ZB
ZB
ZB
W
2.45,I
2.153,I
1.615,I
3.44,D
GaP
GaAs
GaSb
InN
ZB
ZB
ZB
W
2.272,I
1.4241,D
0.75,D
1.89,D
InP
InAs
InSb
ZnO
ZB
ZB
ZB
W
1.344,D
0.354,D
0.230,D
3.44,D
ZnS
ZnS
ZB
W
3.68,D
3.9107,D
ZnSe
ZnTe
CdO
CdS
ZB
ZB
R
W
2.8215,D
2.3941,D
0.84,I
2.501,D
CdS
CdSe
ZB
W
2.50,D
1.751,D
CdSe
CdTe
PbS
PbSe
PbTe
ZB
ZB
R
R
R
—
1.475,D
0.41,D*
0.278,D*
0.310,D*
LATTICE
CONSTANT
(Å)
5.570
3.56683
11.9
5.431073
9.72
4.3596
16.2
5.6579060
ε|| = 5.06 a = 6.6612
ε = 6.85 c = 2.5040
7.1
3.6157
11.
4.5383
—
4.777
ε = 9.14 a = 3.111
c = 4.981
9.8
5.4635
10.06
5.660
12.04
6.1355
a = 3.175
ε||=10.4
ε = 9.5 c = 5.158
11.11
5.4505
13.18
5.65325
15.69
6.09593
a = 3.5446
c = 8.7034
12.56
5.8687
15.15
6.0583
16.8
6.47937
ε||= 8.75 a = 3.253
ε = 7.8 c = 5.213
8.9
5.4102
ε = 9.6 a = 3.8226
c = 6.2605
9.1
5.6676
8.7
6.1037
21.9
4.689
ε = 9.83 a = 4.1362
c = 6.714
—
5.818
ε||=10.16 a = 4.2999
ε = 9.29 c = 7.0109
—
6.052
10.2
6.482
169.
5.936
210.
6.117
414.
6.462
DENSITY
(gm-cm–3)
3.51525
2.329002
3.166
5.3234
2.18
3.4870
2.97
5.22
3.255
2.401
3.760
4.26
6.095
4.138
5.3176
5.6137
6.81
4.81
5.667
5.7747
5.67526
4.079
4.084
5.266
5.636
8.15
4.82
—
5.81
—
5.87
7.597
8.26
8.219
Data are given at room temperature values (300 K).
Key: DI: diamond; HEX: hexagonal; R: rocksalt; W: wurtzite; ZB: zinc blende;
*: gap at L point; D: direct; I: indirect ε||: parallel to c-axis; ε : perpendicular to c-axis
www.eecs.umich.edu/~singh
Bandgaps (in eV) of some semiconductors
TETRAHEDRALLY BONDED MATERIALS
V
C
α-Sn
Si
Ge
C
5.5i,D
Si
2.6i,Z/W
Ge
α-Sn
1.1i,D
0.7-1.1
0.7-1.1i
0.74i,D
III-V N
P
As
Sb
B
Al
Ga
In
2.0i,Z
2.5,Z
2.4i,Z
1.4,Z
1.5i,Z
2.2,Z
1.5,Z
0.41,Z
1.7,Z
0.81,Z
0.24,Z
II-VI O
S
Se
Te
O: Orthorhombic
Zn
Cd
Hg
3.6,Z/W
2.5,Z/W
2.3,T
2.8,Z/W
1.8,Z/W
–.06,Z
2.4,Z
1.6,Z
–.3,Z
Rh: Rhombohedral
I-VII F
Cl
Br
I
distorted rocksalt
Cu
Ag
3.4,Z
3.2i,R
3.1,Z
2.7i,R
3.1,Z
3.0,W
M: Monoclinic
0.09,D
3.8,W
5.9,W
3.5,W
2.4,W
3.4,W
1.3i,R
2.2,O/Rh
2.8i,R
NON-TETRAHEDRAL BONDED MATERIALS
IV-VI compounds
IV-VI O
S
Se
Te
Ge
Sn
Pb
1.7,OR
1.1,OR
0.29,R
1.1,OR
0.9,OR
0.15,R
0.15,R
2.1,R
0.19,R
S
Se
Te
3.6,O
1.9i,T
2.5,M
0.33,T
P
As
Sb
Bi
.33,O
.17,Rh
.10
.015
2.0,i
Group VI elements
VI
Group V elements
V